data_1000051
_cod_database_code               ?
_structure_refined               no
_mpod_phase_name                 Pb(Zn1/3Nb2/3)O3-PbTiO3(0.07)
_chemical_formula_sum            'Pb Nb0.62 Zn0.31 Ti0.07 O3'
_mpod_phase_generic_name         PZN-PT
_mpod_symmetry_point_group_name_h-m 3m
_cell_length_a                   ?
_cell_length_c                   ?
loop_
_publ_author_name
'Zhang R.'
'Jiang B.'
'Jiang W.'
'Cao W.'
_publ_section_title
;Complete set of elastic, dielectric, and piezoelectric coefficients of
 0.93Pb(Zn1/3Nb2/3)O3-0.07PbTiO3 single crystal poled along [011]
;
_journal_name_full               'Applied Physics Letters'
_journal_volume                  89
_journal_issue                   24
_journal_article_reference       242908
_journal_pages_number            3
_journal_year                    2006
_mpod_phase_density              8038.4
_mpod_phase_transition_temperature_rhomb_tetra ?
_mpod_phase_transition_temperature_curie ?
_prop_measurement_poling         '[011]c'
_prop_symmetry_point_group_name_h-m mm2
_prop_frame                      '1=[0-11]c 2=[100]c 3=[011]c'
loop_
_prop_tensorial_index
_prop_dielectric_permittivity_relative_epsrijS
_prop_dielectric_permittivity_relative_epsrijT
_prop_dielectric_stiffness_relative_betrijS
_prop_dielectric_stiffness_relative_betrijT
_prop_elastic_compliance_sijD
_prop_elastic_compliance_sijE
_prop_elastic_stiffness_cijD
_prop_elastic_stiffness_cijE
_prop_electromechanical_coupling_kij
_prop_piezoelectric_dij
_prop_piezoelectric_eij
_prop_piezoelectric_gij
_prop_piezoelectric_hij
_prop_measurement_method
_prop_conditions_frequency
11 . 8240 . 1.2136 . . . . . . . . . CAP 1
22 . 1865 . 5.3619 . . . . . . . . . CAP 1
33 . 3180 . 3.1440 . . . . . . . . . CAP 1
11 6953 . 1.4383 . . . . . . . . . . CAP 10000
22 1847 . 5.4150 . . . . . . . . . . CAP 10000
33 291 . 34.3440 . . . . . . . . . . CAP 10000
11 . . . . 59.4003 67.5153 173.987 145 . . . . . RUS ?
12 . . . . -35.3773 -60.1637 211.639 153.16 . . . . . RUS ?
13 . . . . -16.1684 3.3551 114.275 126.66 . . . . . RUS ?
15 . . . . . . . . 0.4 1823 6.2529 2.49873 1.0158 RUS ?
22 . . . . 26.2949 102.0024 180.240 180.24 . . . . . RUS ?
23 . . . . 5.1644 -54.4683 125.014 150 . . . . . RUS ?
24 . . . . . . . . 0.1 50 3.2360 0.30280 1.9791 RUS ?
31 . . . . . . . . 0.35 478 -8.6446 1.69770 -33.5315 RUS ?
32 . . . . . . . . 0.86 -1460 -17.4399 -5.18545 -67.6476 RUS ?
33 . . . . 15.0523 62.0233 146.292 141 0.87 1150 3.6935 4.08443 14.3266 RUS ?
44 . . . . 15.2998 15.4512 65.360 64.72 . . . . . RUS ?
55 . . . . 245.9933 291.5452 40.65 34.3 . . . . . RUS ?
66 . . . . 14.0845 14.0845 71.000 71 . . . . . RUS ?
